New materials for strengthening and seismic upgrading ... New materials for strengthening and...
Embed Size (px)
Transcript of New materials for strengthening and seismic upgrading ... New materials for strengthening and...
New materials for strengthening and seismic upgrading interventions, International Workshop Ariadne 10, Arcchip, April 22-28 2002, Prague, Czech Republic, cd-rom, 1-24.
New materials for strengthening and seismic upgrading interventions
Antonio Borri University of Perugia, Department of Civil and Environmental Engineering, Via Duranti, 93 06125 Perugia, Italy Marco Corradi University of Perugia, Department of Civil and Environmental Engineering, Via Duranti, 93 06125 Perugia, Italy Andrea Vignoli University of Florence, Department of Civil Engineering, Via di S. Marta, 3 50139 Florence, Italy
1. Abstract This paper focuses on the use of Fiber Reinforced Polymers (FRP) for strengthening and
seismic upgrading interventions applied to existing wood and masonry structures. In order to study the performance of wood beams strengthened with FRP materials, several un-strengthened specimens and beams were tested under four point bending up to the point of failure. Other wood specimens and beams were strengthened with externally bonded carbon, glass or aramidic fiber-reinforced polymer (respectively CFRP, GFRP and KFRP) sheets. The second part of the investigation relates to the interventions on masonry buildings. The results of tests carried out on masonry elements show that the application of FRP materials may provide increases in tensile and shear strength. The use of carbon and glass FRP as a reinforcing method for different kinds of masonry elements (vaults, arches, walls, cells, etc) as well as the different possible positions of the FRP sheets, is analyzed, and some solutions are proposed to avoid peeling problems, increase the value of strength and the efficiency of the bond surface. Experimental results are reported along with the case history of the Town Hall of Assisi, where useful indications were obtained on the practical strengthening operations of the masonry vaults. It is therefore important to recognize that the study and the arrangement of the bonding is the key to optimize the structural behavior of strengthened wood and masonry elements. 2. Introduction
Many un-reinforced wood and masonry structures are widely present throughout Italy and other regions around the world. These structures seem to suffer the most severe damage during earthquakes. Not only the prohibitive cost of replacing all substandard structures, but also the conservation of the historic heritage of the country, necessitates the development of innovative techniques for rehabilitating deteriorating structures. As a consequence most of these structures need strengthening or seismic upgrading work in order to ensure their conservation and functional use. Table 1 shows the possible applications of FRP materials for strengthening and seismic upgrading interventions.
TABLE 1: Possible interventions using FRP materials
Type of intervention using FRP materials
Flexural reinforcement of wood beams using FRP sheets and re-bars epoxy-bonded or inserted in wood-beams in tension zone; Shear reinforcement of wood beams
Shear reinforcement of masonry walls using FRP sheets epoxy-bonded to masonry walls or embedding FRP re-bars mounted near the surface of masonry walls; Flexural reinforcement of masonry walls Seismic upgrading intervention on masonry vaults using FRP sheets; Confinement of masonry columns with FRP sheets; Provisional intervention in order to put in security damaged masonry buildings; Connection of multiple leaf masonry walls (re-bars).
Adhesion between FRP materials and wood/masonry surface; Aging behavior of reinforcement and adhesion; High and low temperatures behavior; Connections of different shapes of FRP materials; Dynamic behavior of the reinforced structures; Types of mortars used in order to leveling masonry surfaces to which the FRP sheets are bonded; Creep behavior; Monitoring methods of reinforced structures (adhesion faults, decreases in mechanical properties of new material, etc)
3. Innovative materials applied on wood structures 3.1 Introduction
The use of composite materials to reinforce wood elements is not new. Tendons for prestressed elements were developed by Rubinsky and Rubinsky (1954)  and by Kaifasz (1960) . High-strength lightweight cables for applications on cable-supported structures, like bridges, were studied by Meier (1987) . Fujisaki et al (1987)  and Saadatmanesh and Ehsani (1989)  analyzed the possibility to replace the steel classically used as a reinforcement in concrete structures by composite rebars, and demonstrated that the response of these materials under load can be predicted using the analytical methods known to practical engineering. The greatest advantage of these materials was their resistance to corrosion.
Ranisch and Rostasy (1986) , and Saadatmanesh and Ehsani (1989)  analyzed the possibility to increase the strength of existing structural members with epoxy-bonded fiber-composite sheets. This application involved external bonding of thin fiber reinforced composite sheets on the tension face of beams using epoxy resins. These studies demonstrated that monodirectional composite sheets are ideal tension reinforcements, and that they provide an important increase in the stiffness characteristics of a structure. Triantafillou and Deskovic (1991)  developed this methodology analyzing the effects obtained by pretensioning the composite sheets before gluing them on the tension face of the beams. They also proposed to apply this technique to increase the strength of existing wood structural members. Before this,
all the studied techniques were applied only in the case of concrete and reinforced concrete structures.
Plevris and Triantafillou (1992)  focused on the development of a fundamental understanding of the behavior of the fiber reinforced wood systems. They examined the effect of external bonding of composite materials on the failure mechanisms, the stiffness, and the ductility of the hybrid member subjected to a combination of bending and axial loads. Thanks to an incremental numerical procedure they concluded that even very small area fractions of fiber-composite reinforcement result in significant improvements of the member's mechanical behavior. Because this technique allows the structural recovery of also very deteriorated wood, it represents a very interesting possibility for all these country where old and historic monuments are common, which is the case of Italy.
In this section the results of a systematic series of tests on reinforced and non-reinforced wood elements are presented. Three different types of wood, different types of fiber reinforced composite materials (FRP), and samples having different geometry have been used. Samples realized using a technique allowing a pretensioning of the composite sheets have been also tested. The results obtained demonstrated that external bonding of composite materials on wood elements, results in significant improvements of the member's mechanical behavior.
3.2 Materials and experimental procedures
3.2.1 Materials Chestnut wood (Castanea Vesca), oak wood (Quercus Cerris) and fir wood (Abies Alba)
have been used for the experimentation. About chestnut and oak, very old woods obtained from ancient buildings situated in central Italy (Umbria), and classified as 1st type wood (wood having very low percentage of defects) , have been used. About fir, wood classifiable as 3rd type wood (wood having diffused defects) has been used.
The hygrometric conditions of these materials have been measured according to the UNI 9091/2 standards ; the humidity percentage resulted equal to 9%, 11% and 15% respectively for chestnut, oak and fir woods. The density of these woods resulted respectively equal to 5.40, 8.98 and 4.24 kN/m3.
The composite reinforcements have been realized using three different types of fibers produced by MAC spa, respectively carbon (CFRP), glass (GFRP) and aramidic fibers (KFRP), having the physical and mechanical characteristics reported in Table 2 as furnished by the producer. Depending on the wood used, small samples or large beams were tested. In the fist case 400 mm long 20 mm large fiber sheets have been used. In the second case 1900 mm long 70 mm large fiber sheets have been used. In the two cases, the thickness of the dry plies was 0.165, 0.118 and 0.070 mm respectively for carbon (CFRP), glass (GFRP) and aramidic fibers (KFRP).
TABLE 2: Mechanical characteristics of the reinforcements (as reported by the producer)
Carbon Fibres Aramidic Fibres E Glass Fibres Aerial density Ds, [Kg m-2] 0.300 1440 0.300 Ply equivalent thickness, [mm] 0.165 0.070 0.118 Tensile Strength, [MPa] 3430 3150 1550 Tensile Youngs modulus, [MPa] 230000 105000 75000 Strain at failure, % 1.5 3.0 2.1
In order to glue composite and wood, a system composed of two curing at room temperature
epoxy resins, primer and saturant, has been used. The mechanical and physical characteristics of these materials are reported in Table 3 as furnished by the producer.
TABLE 3: Mechanical properties of the epoxy resins (as reported by the producer) Primer Saturant Tensile Strength (ASTM D638) >12 MPa >50 MPa Tensile Strength from bending test (ASTM D790) >24 MPa >120 MPa Compression Strength (ASTM D695) - >80 MPa Elongation at break, % (ASTM D638) 3.0 2.5 Flexural Youngs modulus (ASTM D790) >580 MPa >3500 MPa Tensile Youngs modulus (ASTM D638) >700 MPa >3000 MPa
The gluing procedure consisted, as a first step, in straining the primer on the wood surface
where the reinforcement had to be placed. After the partial polymerization of this la